VIEWS: 79 PAGES: 4 CATEGORY: Consumer Electronics POSTED ON: 2/6/2011
TFT (Thin Film Transistor) LCD, which is an active matrix type liquid crystal display (AM-LCD) in one. LCD flat panel displays, in particular TFT-LCD, is the only brightness, contrast, power, life, size and weight to catch up and fully integrated performance than CRT display device, and its excellent performance characteristics of a good large-scale production high degree of automation, low-cost raw materials, the development is vast, and will quickly become a mainstream product in the new century, global economic growth in the 21st century, a bright spot.
ESSDERC 2002 An Ultra-Thin Polycrystalline-Silicon Thin-Film Transistor with SiGe Raised Source/Drain Du-Zen Peng, Po-Sheng Shih, Hsiao-Wen Zan, Ta-Shun Liao, Chun-Yen Chang Institute of Electronics, National Chiao Tung University, Hsin-Chu, Taiwan firstname.lastname@example.org SiGe raised source/drain structure is proposed. The new Abstract device characterizes a thin active channel region and a thick SiGe source/drain region. The raised source/drain An ultra-thin poly-Si thin film transistor (poly-Si region is self-aligned to poly-gate and no additional TFT) with SiGe raised Source/Drain (SiGe RSD) was mask is needed in comparison with conventional TFTs. fabricated. The raised source and drain regions were Comparison of experimental Id-Vg characteristics, on/off selectively grown by ultra-high vacuum chemical vapor current ratio, and breakdown voltage for the proposed deposition (UHVCVD) at 550°C. The resultant novel structure and conventional thin-layer TFTs are transistor has an ultra-thin channel region with reported. thickness of 20 nm and a self-aligned thick S/D region, which leads to better performance. With this structure, 2. Experimental the turn-on current in the I-V characteristics increases dramatically and the drain breakdown voltage is The key fabrication steps of the proposed SiGe raised increased as well, compared with conventional thin- Source/Drain device are shown in Figure 1. Silicon channel poly-Si TFTs. wafers coated with a 500nm thermal oxide were used as the starting substrates. A 20nm undoped ultra-thin 1. Introduction amorphous-Si (a-Si) layer was deposited by low- pressure CVD (LPCVD) at 550°C. The deposited a-Si Polycrystalline silicon thin-film transistors (poly-Si TFTs) are attractive for many applications, such as the Poly-SiGe Oxide Sapcer switching devices as well as peripheral driving circuits Poly-SiGe Poly-SiGe in the active matrix liquid crystal display (AMLCD) , . In order to integrate peripheral driving circuits on Poly-Gate the same glass substrate, both a large current drive and a high drain breakdown voltage are necessary for poly-Si Gate Oxide TFT device characteristics. There were papers indicating Poly-Si that thinning the active channel film is beneficial for Oxide obtaining a higher current drive [3-5]. However, the use of thin active channel layer inevitably results in poor source/drain contact and large parasitic series resistance. Figure 1. Key process steps with cross-sectional In addition, the short-channel poly-Si TFTs also suffer schematic for SiGe raised S/D poly-Si TFTs. from a low drain breakdown voltage, which cannot meet the driving requirement for the thin active channel layer was then recrystallized for 24 h in nitrogen devices. An ideal TFT device structure should therefore ambient at 600°C. After patterning and plasma etching consist of a thin active channel region, while to form the active device island, a 50 nm gate oxide was maintaining a thick source/drain region. The thick deposited by plasma-enhanced CVD (PECVD) at 300°C. source/drain region has the advantage of not only This was followed by the deposition and patterning of a reduction of the lateral electric field near drain side, thus 300 nm poly-Si gate layer. A 300 nm TEOS oxide was maintaining the drain breakdown voltage , , but then deposited by PECVD, and anisotropically etched by also reduction of the source/drain series resistance. reactive ion etching (RIE) to form a sidewall spacer However, previous methods [6-7] used to fabricate such abutting the poly-Si gate. The remaining TEOS oxide structures with thin active channel and thick source/drain above the source and drain regions was removed in region require one or more additional masks, and are not diluted HF to ensure the exposure of the S/D poly-Si self-aligned in nature, when compared to the region. Afterwards, some wafers were loaded into a conventional TFTs. UHVCVD system to selectively grow an undoped SiGe In this experiment, a novel TFT with self-aligned layer on the exposed source, drain and gate regions at 535 550°C. The growth of SiGe on source, drain and gate the I-V curves behave more like resistance. The total regions was inherently self-aligned. The thickness of the resistance (Rtotal) from drain to source is a composition SiGe was about 100 nm. Figure 2 shows a cross- of source/drain (RS/D) and channel (Rchannel) resistance, sectional TEM photo of the fabricated structure. Next, which can be expressed as the following equation: the gate electrode and source/drain regions were Rtotal = 2RS/D + Rchannel. implanted by phosphorus ions at a dosage of 5×1015cm-2, With the ultra-thin source/drain region, the and an energy of 55 keV. For comparison, wafers with conventional TFT suffers from a high RS/D. So when the conventional TFTs were also processed on the same run gate bias increases, the output current is subject to be by deliberately skipping the growth of SiGe and using a phosphorus implant energy of 15keV instead. All wafers limited by the source and drain resistance (RS/D), as shown in Figure 4. In contrast, due to its thick were then subjected to a RTA anneal at 850°C for 20 source/drain region, the RS/D is much smaller for SiGe- seconds for dopant activation. The measured resistivities RSD TFT. As a result, the output current is not limited were 2×10-3 Ω-cm and 4.6 Ω-cm for SiGe raised S/D by the parasitic source/drain resistance, and therefore is and conventional TFTs, respectively, indicating that a much larger than that of the conventional TFT. significant reduction in S/D resistance was indeed obtained by using a thicker S/D film. Next, a 300 nm- 10-4 W/L=10µm/10µm thick oxide was formed as the cap layer by PECVD. 10-5 Vd=5V Finally, contact hole definition and Al metallization Conventional, Vd=0.1V Conventional, Vd=5V were performed, followed by a 400°C sintering in 10-6 SiGe RSD, Vd=0.1V nitrogen ambient for 30 minutes. 10-7 SiGe RSD, Vd=5V Id (A) 10-8 Vd=0.1V 10-9 10-10 10-11 10-12 -5 0 5 10 15 20 25 30 Vg (V) Figure 3. Comparison of Id-Vg characteristics of SiGe raised S/D TFTs and conventional poly-Si TFTs 2.5 8 Conventional SiGe RSD Vg=25V 7 2.0 Id (µA), Conventional W/L=10µm/10µm Id (µA), SiGe RSD 6 Figure 2. Cross-sectional transmission electron 1.5 5 microphotograph (TEM) of a fabricated SiGe raised 4 S/D TFT. The thickness of the SiGe on 1.0 Vg=20V 3 source/drain region is approximately 100 nm. 2 0.5 1 3. Results and Discussion 0.0 0 0 2 4 6 8 10 12 14 16 18 Figure 3 shows the comparison of typical Id-Vg Vd (V) characteristics for the conventional and the proposed Figure 4. Comparison of Id-Vd output characteristics SiGe raised S/D TFTs. It can be seen that the turn-on of SiGe raised S/D TFTs and conventional poly-Si characteristics are significantly improved for SiGe raised TFTs. S/D TFTs. Approximately one order of magnitude improvement in the on/off current ratio is observed for The scaling of channel dimensions in poly-Si TFTs is SiGe raised S/D TFT, as compared to the conventional critical to realize high density AM-LCD with integrated TFTs. The larger leakage current for conventional TFTs driver circuits on the same glass panel. To this end, the is probably due to the stronger horizontal electric filed drain breakdown voltage requirement must be satisfied. near drain side, which results in smaller breakdown Figure 5 shows the drain breakdown voltage, which is voltage for conventional TFTs, as will be discussed later. defined arbitrarily as the drain voltage when the drain Figure 4 depicts the output characteristics for both SiGe current equals 2 nA with Vgs = 5V, for both the raised S/D and conventional TFTs. It can be seen that for conventional and SiGe-RSD TFTs. It can be seen from the conventional TFTs, as the gate voltage gets higher, Figure 5 that for mask length (Lg) changing from 10 µm 536 to 1 µm, the breakdown voltage for conventional TFTs experimental data show that the new SiGe raised S/D decreases from 10.7 V to 5.3 V (50%), while only 12% poly-Si TFT has higher turn-on current and on/off of difference (from 16.1 V to 14.2 V) in breakdown current ratio in comparison with the conventional TFTs. voltage is observed for SiGe RSD TFTs. The larger Moreover, the drain breakdown voltage for SiGe raised breakdown voltage for SiGe-RSD TFTs can be S/D poly-TFTs is significantly improved for smaller gate attributed to the thicker source/drain region and hence length. The new structure is therefore ideally suitable for smaller horizontal electric field near the drain side , implementing high-density and high-performance driver . This result is also consistent with the larger leakage circuits on the glass panel for AM-LCD applications. current observed in Figure 4 for conventional TFTs with Lg = 10 µm. 5. References 18  H. Oshima and S. Morozumi, “Future trends for TFT integrated circuits on glass substrates,” in IEDM Tech. Dig., 16 1989, pp. 157-160. Breakdown Voltage (V) 14  S. D. Brotherton, “Polycrystalline silicon thin-film transistors,” Semicond. Sci. Technol., vol. 10. pp. 721-738, 12 1995.  T. Naguchi, H. Hayashi, and T. Oshima, “Low temperature 10 polysilicon super-thin-film transistor (LSFT),” Jpn. J. Appl. Phys., vol. 25, no. 2, pp. L121, 1986. 8 W=10µm  M. Miyasaka, T. Komatsu, W. Itoh, A. Yamaguchi, and H. 6 Conventional Ohashima, “Effects of channel thickness on poly-crystalline SiGe RSD silicon thin film transistors,” Ext. Abstr. SSDM, pp. 647-650, 4 1995. 2 4 6 8 10  M. Yoshimi, M. Takahashi, T. Wada, K. Kato, S. Gate Length (µm) Kambayashi, M. Kemmochi, and K. Natori, “Analysis of the drain breakdown mechanism in ultra-thin-film SOI Figure 5. Id-Vg curves as a function of different gate MOSFET’s,” IEEE Trans. Electron Devices, vol. 37, pp. 2015- length (Lg) from 10 µm to 1 µm for conventional 2020, Sept. 1990. TFTs and SiGe raised S/D TFTs.  A. Kumar, J. K. O. Sin, C. T. Nguyen, and P. K. Ko, “Kink-Free Polycrystalline Silicon Double-Gate Elevated- Channel Thin-Film Transistors,” IEEE Trans. Electron Devices, vol. 45, pp. 2514-2520, Dec. 1998. 4. Conclusion  S. Zhang, C. Zhu, J. K. O. Sin, and P. K. T. Mok, “A We have proposed an ultra-thin poly-Si TFT with Novel Ultrathin Elevated Channel Low-Temperature self-aligned SiGe raised source/drain structure. The Poly-Si TFT,” IEEE Electron Device Lett., vol. 20, proposed structure was successfully fabricated without pp.569-571, Nov. 1999. additional masks and is self-aligned in nature. Our 537 538
Pages to are hidden for
"An Ultra-Thin Polycrystalline-Silicon Thin-Film Transistor with "Please download to view full document